Embed Size (px)
Transcript of Glass Ceramics
ME 3701, Material of Engineering Laboratory, LSU1
The primary objective of this study is to gain an understanding of the mechanical properties, and underlyingatomic structures that cause the properties, of ceramic materials through application of Modulus of Rupture tests.
The primary drawback of using ceramic materials in structural applications is their inherent brittleness whichresults from strong bonding coupled with electrical balancing restrictions due to the metallic plus non-metallicnature of ceramic compounds. The Modulus of Rupture (MOR) test is the standard for determining themechanical properties of ceramics (Flexural Strength and Flexural Modulus). Variations in Flexural Strengthas a function of firing temperature and specimen size will be examined experimentally (MOR) and evaluatedusing the statistical t-test; large ceramic parts generally have lower strengths due to their higher probability ofcontaining critical flaws.
Ceramics are generally composed of Metallic + Non-Metallic Compounds which are primarily IonicallyBonded.
Silicon and Oxygen are Common in Ceramics due to Availability and Cost.
Common Structural Ceramics include Silicon Oxides, Nitrides and Carbides which include clay minerals suchas pottery, tiles, cement and glass.
General Ceramic Properties:
Insulative, Refractory, Hard and Brittle.
Advanced Ceramic Applications:
Tools for Machining Hard Metallics.
Coatings that Require High-Temperature Resistance and Chemical Stability (Enamels).
Optical uses include: Lasers, Florescent Screens and Iridescent Films.
Brittleness is the Primary Drawback of Ceramics; Ceramic Compounds are being developed which exhibitmeasurable ductility with excellent strength and hardness.
Three General Categories of Ceramics:
1. Crystalline Ceramics include Silicates, Oxides and Non-Oxide Compounds which form crystallinesolids and are utilized in pottery, bricks and many high-tech industries such as aerospace andelectronics.
2. Glasses include Silicate and Non-Silicate Compounds which are non-crystalline; Glasses aregenerally Amorphous.
3. Glass-Ceramics are composed of crystalline ceramics that are initially formed as glasses and aresubsequently crystallized under controlled thermal processing.
ME 3701, Material of Engineering Laboratory, LSU2
Figure 1 - (a) Crystalline Ceramic Structure, (b) Amorphous Ceramic Structure. [Askeland, 1996]
Most Crystalline Ceramics are SiOi2 based and are termed Silicates.
Silicate Examples: Pottery, Whiteware, Bricks, Tile.
Table 1 - Compositions of some Silicate Ceramics. [Shackelford, 1992]
Note that Silicate Ceramics are generally Oxides!
Crystalline Ceramic Formation involves Firing which refers to controlled heating that Dries and Facilitates IonicBonding of the Compounds.
Ceramic Strength is highly dependent on Porosity (size and number of voids) which act as crack initiation sites.Crystalline Ceramics are influenced by the Nature of the Component Ions:
Crystals must be Electrically Balanced thus Compositions must be Balanced! Relative Ion Size generally determines the Crystalline Structures that form.
Due to Electrical Balancing restrictions, Crystalline Imperfections occur in Pairs:
Schottky Defects - Vacancy Pair (Cation & Anion) Frenkel Defects - Cation Vacancy near a Cation Interstitial
ME 3701, Material of Engineering Laboratory, LSU3
Figure 2 - Illustrations of Frankel and schottky defects. [Callister, 1991]
Electrical Balancing Restrictions are also partially responsible for Ceramic Brittleness; Dislocation Movement andPlastic Deformation are minimal.
Figure 3 - Sample Ceramic Crystal Unit Cell Structures. [Callister, 1991]
Pure Oxide Compounds with very small impurity levels, such as BaTiO3, make excellent high-endsemiconductors but are relatively expensive.
Non-Oxide Ceramics, such as Silicon Carbide and Boron Nitride, include refractories and abrasives which aredeveloped for heat and wear resistance.
Ordinary sand is primarily SiO2 which is utilized to produce window glass.
Most Glasses are produced by the addition of oxides, such as CaO and Na2O, which catalyze the formation ofrandom 3-D networks of SiO2 .
ME 3701, Material of Engineering Laboratory, LSU4
Table 2 - Compositions of some Silicate Ceramics. [Shackelford, 1992]
Examples of Common Non-Crystalline Ceramics
Vitreous Silica is relatively pure SiO2 which can withstand temperatures up to 1000oC; typically utilized in
E-Glass and S-Glass are thin pultruded fibers utilized in Composites.
Enamel is a ceramic coating applied for Temperature & Corrosion Protection.
Window Glass is a mixture of Oxides; 72% SiO2 with Na2O, CaO, MgO and Al2O3.
Glass Ceramics are a new group of materials which are initially relatively ordinary glassware which is cheap andeasy to form.
90% of the glassy material can be Crystallized though controlled heat treatment; small-grained, nearly pore-freeceramics form which are Strong and Shock Resistant.
Crystallization is a Nucleation and Growth process; catalysts are added to facilitate the formation of numerousgrains.
Table 3 - Compositions of some Glass Ceramics. [Shackelford, 1992]
Figure 4 - Photograph of a partially crystallized Glass-Ceramic. [Smith,1993]
ME 3701, Material of Engineering Laboratory, LSU5
Bend Test - Modules of Rupture
In ductile materials, the stress-strain behavior is found by applying the tensile test (as determined in previousexperiments). The curve typically goes through a maximum which is where the tensile strength is located.Failure occurs at a lower stress after necking has reduced the cross-sectional area supporting the load. Onthe other hand the stress-strain behavior of brittle ceramics is not ascertained by a tensile test. There aremany reasons the tensile test is not used:
1. it is difficult to prepare and test specimens having the required geometry;
2. it is difficult to grip brittle materials without fracturing them;
3. surface flaws often cause premature failures; and
4. ceramics fail after only about 0.1% strain thus specimens must be perfectly aligned in order toavoid the presence of bending stresses.
For these reasons a more suitable transverse bending test is used.
In the bend test (or flexure test) a bar specimen having either a circular or rectangular cross section is bentuntil fracture using a three or four point loading technique.
Figure 10 - (a) The bend test often used for measuring the strength of brittle materials, and (b) the deflection dobtained by bending. [Askeland, 1994]
At the point of loading, the top surface of the specimen is placed in a state of compression and the bottom surfaceis in tension. Stress is computed from the specimen thickness, the bending moment, and the moment of inertia ofthe cross section. The maximum tensile stress exists at the bottom surface of the center of the specimen, directlybelow the point of load application. Since the tensile strengths of ceramics are about one-tenth of theircompressive strengths and fracture occurs on the tensile specimen face, the bend test is a valid substitute for thetensile test.
Figure 11 - The stress-strain behavior of brittle materials compared with thatof more ductile materials. [Askeland, 1994]
ME 3701, Material of Engineering Laboratory, LSU6
For a 3-point bend test of a rectangular bar, the stress at fracture using the bend test is known as the FlexuralStrength or Modulus of Rupture and is given by
Where fs = Flexural Strength
F = Fracture Load
L = Length Between Outer Supports
w = Specimen Width
h = Specimen Height
The results of the bend test are similar to stress-strain curves; however the stress is plotted versus deflectionrather than versus strain.
Figure 12 - Stress-deflection curve for MgO obtained from a bend test. [Askeland, 1994]
The modulus of elasticity in bending, the flexural modulus, is determined from the linear portion of the Stress-Deflection curve and is given by
Because cracks and flaws tend to remain closed in compression, brittle materials are generally designed suchthat only compressive stresses act on the part.
Efs = Flexure Modulus
= Beam Deflection
F1 = 2/3 Fmax with 1 @ 2/3 Fmax
F2 = 1/3 Fmax with 2 @ 1/3 Fmax
ME 3701, Material of Engineering Laboratory, LSU7
t-Test for Determination of Mean Differences
There is often considerable variation and scatter in flexural strength for many specimens of a specific brittleceramic material. This phenomenon may be explained by the dependence of flexural strength on theprobability of the existence of a flaw that is capable of initiating a crack. This probability varies from specimento specimen of the same material and depends on fabrication technique and any subsequent treatment.Specimen size also influences flexural strength; the larger the specimen, the greater the probability of criticalflaw existence, and the lower the flexural strength. The t-Test is a statistical method that is applied todetermine whether or not significant mean differences exist between two sets of repeated measures data.The method will be applied to determine whether or not a specimen size effect is evident in the Modulus ofRupture tests being conducted in this experiment.
A small sample-size test (less than 30 measurements) of the significance of